Zvonimir Janović, Ante Jukić, Otto Vogl* University of Zagreb, Faculty of Chemical Engineering and Technology * University of Massachusetts, Department of Polymer Science and Engineering
Spacer groups in macromolecular structures
Razmakne skupine u strukturi makromolekula
Author’s Review / Autorski pregled
Razmakne skupine bitna su odrednica strukture i svojstava funkcijskih polimera. Mnoga ﬁzička, kemijska i biološka svojstva znatno ovise o njihovoj veličini. Određuju elastičnost i preradljivost vrlo krutih polimernih sustava, sklonost kristalizaciji temeljnih i bočnih skupina, kemijsku reaktivnost funkcijskih skupina, kao i mnoga druga svojstva. U biološkim makromolekulama elastičnost razmaknih skupina odgovorna je za stabilnost polipeptidnih struktura. Tijekom vlastitih istraživanja određen je utjecaj razmaknih skupina većeg broja sintetskih polimera, posebice polialdehida, poli(oksi-etilena), polioleﬁna, poli(estera ω-alkanskih kiselina) i poli(alkil-metakrilata) na sklonost kristalizaciji bočnih skupina i kemijsku reaktivnost. Prikazan je utjecaj kratkolančanih razmaknih skupina na stereospeciﬁčnu orijentaciju monomernih molekula prema aktivnim koordinacijskim katalitičkim centrima i nastajanja kristalnih izotaktnih struktura na primjeru polimerizacije polipropilena.
Received / Primljeno: 21. 12. 2009. Accepted / Prihvaćeno: 19. 4. 2010.
Abstract Spacer groups are often an essential part of polymer structures, particularly functional polymers. Many physical, chemical and biological properties depend strongly on their size. They provide ﬂexibility and fabricability in highly rigid polymers. They also provide accessibility of functional groups, crystallization of side chains, separation of groups from the main chain for efﬁcient chemical reactions and other characteristics. They can be found in natural polymers where ﬂexible spacer groups provide essential links for the stability of polypeptide structures. In our research work we have studied the effects of ﬂexible side chains for side chain crystallization and ﬂexible side groups for reactivity on synthetic polymers, particularly, polyaldehydes, polyoleﬁns, poly(ethylene oxides), poly(ω-alkenoic acid esters) and poly(alkyl methacrylates). Ultimately, we have shown some interest in how ﬂexible links behave because of their oligomeric nature. The importance of short spacer groups on the crystallization of stereoregular polymers could possibly inﬂuence the stereospeciﬁcity of the addition to the catalyst site, for example, in propylene polymerization. In this paper we are trying to show, on a few demonstrative examples, the importance of spacer groups in macromolecular structures. KEY WORDS: functional polymers polyaldehydes poly(alkyl methacrylates) poly(ethylene oxides) polymer structure polyoleﬁns poly(ω-alkenoic acid esters) spacer groups KLJUČNE RIJEČI: funkcijski polimeri polialdehidi poli(alkil-metakrilati) poli(esteri ω-alkanskih kiselina) polimerna struktura poli(oksi-etileni) polioleﬁni razmakne skupine 14
Introduction Polymers with functional groups are of great interest, because they impart speciﬁc chemical, spectroscopic and mechanical polymer properties. Many have been synthesized where the active groups are liquid crystals, catalysts for chemical reactions or hydrogenations. Polymeric UV absorbers, antioxidants, polymers with photo-, thermo- and electro-active as well as biologically active groups1 have also been prepared. Such polymers may include homopolymers and copolymers, polymers of various additional characteristics: speciﬁc solubility, swellability or even completely insoluble materials; they also include oligomers or polymers of low, medium and high molecular, or specially designed molecular weights or molecular weight distributions. Functional polymers have been prepared in order to modify such basic chemical and physical properties as glass transition temperature, melting point, solubility, crystallinity and other fundamental properties, which depend directly upon steric requirements, polarity and interaction of functional groups. It has been estimated that polymers in the health and food industry and for the production and preservation of energy, will be the main thrust of the research development in polymer science over the next decade; as polymer engineering, polymer physics and polymer chemistry, respectively, were important in the development of polymer science in each of the preceding decades. In this discussion examples of spacer groups inﬂuence on properties of some typical functional polymers based mostly on our own research activities are presented. Spacer groups provide accessibility of functional groups, crystallization of side chains, separation of groups from the main chain for efﬁcient reactions and other characteristics. They can be found in natural polymers where ﬂexible spacer groups provide essential links for the structure conﬁguration and stability of polypeptide structures. There has been tremendous attention paid to the inﬂuence of the kind and size of spacer groups. The reactivity of a functional group may be low when it is directly attached to the main chain, which may be a result of steric hindrance by the polymer backbone and neighboring side groups. Vogl and others2,3 described the effect of spacer groups in different POLIMERI • 31 (2010) 1:14-21
applications separating the functional groups from the backbone chain. Spacer groups may be either ﬂexible or stiff. In general, they provide ﬂexibility and allow the reactive group to react independently from the main chain. Thus, liquid-crystalline, mono-substituted acetylenes containing terphenyl pendent groups with methylene groups of varying spacer lengths and their polymers were synthesized.4 The polymer with long spacers (hexamethylene), formed a nematic mesophase when heated and cooled; however, the polymer with short spacers (methylene) could not exhibit liquid crystallinity at elevated temperatures. G. Luckhurst5 has employed the molecular ﬁeld theory to predict the variation of the transitional properties of liquid crystal cyanobiphenyl dimers with the length of the spacer. He found that for spacers containing about 12 or more atoms, the odd-even effect predicted for the transitional properties varies signiﬁcantly depending on the model used to describe the spacer conformation; that is, whether the torsional angles deﬁning the conformations is taken to be discrete or continuous. In recent years, there have been intense efforts to develop methods to recover and reuse homogenous catalysts.6 Among these methods; the use of low molecular weight soluble linear polymers or dendrimers as supports have become attractive approaches since the supported catalysts are in the same phase as the reactants. In order to increase the accessibility of the catalytic sites, a spacer is often placed between the soluble polymer and the catalyst. The spacer units are mostly chosen to suit the chemistry of the end group on the polymer. It was shown that the reactivity and selectivity of this type of polymersupported catalyst is dependent on the nature of the spacer.
Natural polymers Nature has carefully selected spacer groups in their polymer structures and for our life. Nucleic acids are polyphosphoric acids, which are linked by pentoses to the bases of purines, and pyrimidines that ultimately form the double helix. Proteins are convincing examples of how ﬂexible spacers, methylene spacer groups, dominate the conformation of the tertiary and quaternary structure of large protein molecules.7 Most consist of complicated structures, β-helices of poly(α-amino acids) connected with random α-amino acid chains (Fig. 1). The α-amino acid units have spacer groups, methylene units, between the peptide chain and the functional group: i) a carboxylic group in glutamic acid, ii) an amino group in lysine and ornithine, and iii) a short hydrocarbon chain in leucine and isoleucine (whose function is to provide the hydrophobic interactions that stabilize secondary structure in proteins). The stunning discovery of Kauzman in the 1950s showed that hydrophobic portions for the macromolecule, such as leucine, isoleucine and phenylalanine interact and are capable of associating in hydrophobic clusters (Fig. 2).8 They are substantially responsible for the fragile poly(α-amino acid) structures in aqueous medium in the region of 37°C ± 10°C, in which we exist; above this temperature, denaturation of the proteins occurs.9
FIGURE 1 – Typical helical structure of protein molecule7
Some of the basic amino acid units have functional groups, such as amino, thio, and carboxylic acid groups. They are attached to the chiral a-carbon atom of the amino acid with 2 or 4 methylene units. Examples are lysine, ornithine, arginine, threonine and glutamic acid. Having the advantage of ﬂexible links, they are now free to interact with other parts of the macromolecule, not necessarily with one in the vicinity. Of the 20 protein amino acids, 16 have a methylene group at the b- position, and a further three bear a methine group. No aromatic, carboxamido-, carboxylic carbon, or heteroatoms are attached directly to the α-carbon atom, but they are separated by this methylene or occasionally by a longer n-alkylene spacer group. The appearance of and the role played by the spacer group are discussed in an evolutionary context. P. Tompa10 by studying the role of a spacer group in the protein amino acid, has concluded that the general role of the spacer group is to ensure the uniformity of the constant regions H2N-CH-[(CH2)n-R’]-COOH and the individuality of the R’ contact groups by spatially separating them. Polysaccharides, carbohydrates, are used for nutritional purposes such as cellulose, starches and sugars. To prevent water from evaporating from fruits and vegetables, the skin of several fruits and vegetables are composed of esters of high aliphatic fatty acids of cellulose. Examples of such fruits are apples, pears, and cherries and of such vegetables tomatoes, peppers and cucumbers.
Side chain crystallization Isotactic polyaldehydes Isotactic polyaldehydes crystallize in helical conformations in different helices, depending on the size of spacing groups. Polyformaldehyde (polyoxymethylene) crystallizes in a 21 helical conformation with a
FIGURE 2 – The spacer groups in some selected a-amino acids8
POLIMERI • 31 (2010) 1:14-21
melting point of 178°C. Higher polyaldehydes with linear aliphatic side chains crystallize generally in 41 helices. Polyacetaldehyde melts at 165°C, poly(propionaldehyde) at 185°C and poly(n-butyraldehyde) at 225°C.11,12 The 41 helical crystalline structure for poly(n-heptaldehyde) is shown in Figure 3.13
FIGURE 3 – Helical 41 structure of isotactic poly(n-heptaldehyde)13
FIGURE 5 – Comparison of melting transitions of linear higher aliphatic isotactic polyaldehydes and polyoleﬁns14,17
From poly(n-valeraldehyde), a second transition point is observed, which we have identiﬁed as a transition of crystallization of the parafﬁnic side chain. It occurs in the region of 60-80°C. The higher melting transition in the region of initially 120-150°C is assigned to the melting of the polyacetal helix. The second transition is the transition (melting) of the parafﬁn side chain (Figure 4).14-16 The exact values of the transition (melting points of polyaldehydes and polyoleﬁns) are shown in Figure 5. After poly(n-octaldehyde) the polyacetal melting around 120°C of the initially prepared polymer is no longer observed. But on annealing for a day above the transitions of the parafﬁnic melting transition or after solid-state extrusion, the polyacetal transition shows up clearly as a small but distinguishable transition peak. In addition, in thermal or mechanical treatment, the original peak of the parafﬁnic transition temperature splits into one major and one or two minor peaks, only a few degrees temperature separated, indicating a slightly different crystal alignment of the linear parafﬁnic side chains. After poly(n-nonaldehyde) no more transition temperature peak that could be assigned to the polyacetaldehyde part of the crystalline isotactic polyaldehyde could be observed under any treatment. It should be noted that the polymer of the branched isobutyraldehyde has a high melting point (dec.) of 305°C. This means that bulky side chains of the aldehyde monomer produced an isotactic polymer with a very rigid helix and consequently high melting point. Higher aliphatic aldehydes polymerize well with anionic initiators, such as lithium tert-butoxide below their ceiling temperature (usually below
-40°C) of polymerization and the polymers can be end capped to improve their thermal stability. The polymerization up to now has been limited to n-undecaldehyde because the melting point of the aldehyde is above the low temperature required for polymerization. Once the aldehyde’s melting temperature is above the ceiling temperature of its polymerization it is difﬁcult to induce polymerization effectively. Polymerization of higher aliphatic aldehydes with cationic initiators above the ceiling temperature results in cyclotrimerization to 2,4,6-tri-n-alkyl-1,3,5-trioxanes, crystalline with higher aldehydes. The trimer of n-nonaldehyde melts at 36°C, that of n-decaldehyde at 48°C, n-undecaldehyde at 56°C, and n-dodecaldehyde at 61°C. They all show one sharp transition point. Isotactic polyoleﬁns It was intriguing to compare the transition (melting) points of isotactic polyaldehydes with those of polyoleﬁns.17 Crystalline isotactic polyoleﬁns have a 31 helical structure. Polypropylene melts at 165°C and poly(1-butene) at 126°C. It has several different crystalline forms, some melt as high as 134°C. Linear polyethylene melts at 136°C and is not helical but has an extended chain structure.18 The next few isotactic polyoleﬁns melt at much lower temperatures, apparently because of interactive effects of the longer side chains of the isotactic polyoleﬁns with the main chain of the polyoleﬁn helix. As the length of the side chain of the isotactic polyoleﬁns increases to poly(n-nonene) the melting transition reaches the level of the parafﬁnic side chain transition of the isotactic polyaldehydes. In other words, the melting transitions are determined by the melting transition of
FIGURE 4 – Melting behavior of: (a) isotactic polyaldehydes (b) parafﬁn side chain14
POLIMERI • 31 (2010) 1:14-21
the parafﬁnic side chains. As in the one case of the melting transition of polyaldehydes, isotactic polyoleﬁns with bulky side groups, like poly(3methyl pentene) or poly(3,3-dimethyl butene) have high melting points, in the range of 300°C.
Others It should be mentioned that melting points of polymers in the range of 40-60°C have been recognized by Platé and his group in the early 70s.19 They studied poly(n-dodecyl methacrylate), an atactic polymer as far as the polymer main chain is concerned, and found it to be a crystalline polymer melting around 40°C. Clearly it was a classic example of polymer that was crystalline because it had a linear parafﬁnic side chain that was capable of crystallizing as a parafﬁnic side group. Janovic et al.20 studied side-chain crystallinity in the scope of research of polymeric additives for lubricating mineral oils. It was found that increase of the content of crystalline phase i.e. long-chained alkyl methacrylates in copolymer (Figure 6), lowered the pour point of oil solutions, thus conﬁrming that the side long-chained groups of n-alkyl methacrylate are an active component of the copolymer that reduces the mineral oil pour point. Therefore, the content of crystalline phase may be directly associated with pour point values of mineral oil solutions. The length of the alkyl group in n-alkyl methacrylates also inﬂuenced the monomer copolymerization reactivity and polymerization rate.21-23
from the polymer main chain, crystallization between the main chain and the functional end group, a kind of side chain crystallization can occur, if the spacer group is three methylene groups longer. We have another signiﬁcant observation relevant to the question: How long does the propylene oligomer chain have to be before crystallization can occur? We have carefully studied the embryonic state of the polymerization of trichloroacetaldehyde (chloral).26 Chloral does not directly resemble propylene as the monomer but the initial state of its polymer formation could be readily investigated and we have studied it extensively. The purpose of this study was to understand and establish the inﬂuence of the size (diameter) of the side group (trichloromethyl) on the forced stereospeciﬁcity based on size alone. We found that chloral polymerizes to an exclusively stereospeciﬁc and conformational speciﬁc polymer, with a turn angle of the helix of 97.3° and an 113 helical structure. In the ﬁrst addition of the chloral monomer unit to the (anionic) catalyst, the polymerization is not stereospeciﬁc. The ﬁrst addition is, as expected, a 50:50 addition to the achiral initiator. As further addition of the monomers to the ﬁrst addition products proceeds, the stereochemistry of addition is ﬁrst favored and then forced (without any additional coordinative force) into a stereospeciﬁc and conformational speciﬁc crystalline polychloral. This occurs after the ﬁrst turn of the helix, in other words after the pentamer or hexamer is formed, further addition of chloral is completely stereospeciﬁc and conformationally speciﬁc. We have now two arguments. In the case of the parafﬁn crystallization of polyaldehydes we require ﬁve methylene units before crystallization of the side chain can occur. This, of course is a random parafﬁnic crystallization, as is the case in the crystallization of the higher poly(ω-alkenoates). In the case of embryonic state of chloral polymerization we found that about ﬁve monomer units are needed to begin to form the helix. We would like to call this phase, the amorphous phase. Polymerizations Methyl ω-alkenoates were prepared from commercially available w-alkenoic acids or the ω-alkenoic acids were synthesized (Figure 7).25 The acids were esteriﬁed with methanol in high yields and epoxidized. The epoxidation of the higher ω-alkenoates proceeded in nearly quantitative yield (Figure 8). The relative ease of epoxidation of ω-hexenoate, which is essentially the same as oleﬁn epoxidation has made higher ω-alkenoic acids and their epoxides attractive monomers (Figure 9).27
FIGURE 6 – Crystalline phase content in dependence on styrene / dodecyl methacrylate / octadecyl methacrylate (ST/DDMA/ODMA) or methyl methacrylate / dodecyl methacrylate / octadecyl methacrylate (MMA/DDMA/ODMA) terpolymer composition21,22
The azobenzene monomers containing methacrylate groups varied by having alkyl spacers of varying lengths and, either nitro or methoxy substituents in conjugation with the azo groups, were polymerized via atom transfer radical polymerization (ATRP).24 The kinetics of ATRP for each azo monomer was also studied. The effects of the types of substituents and the length of the spacer of the methacrylate monomers and the effect of molecular weight on the property of polymers were established.
Inﬂuence of spacer groups in functional polymer Polymer structures In our studies of the transitions of polyoleﬁn carboxylates we have particularly concentrated on the parafﬁnic melting transition of poly(ω-hexenoates) and poly(ω-undecenoates). Poly(methyl ω-hexenoate) shows no transition in the 40 to 60°C range but poly(methyl ω-undecenoate) does. This again demonstrates, that, with a sufﬁciently long methylene grouping POLIMERI • 31 (2010) 1:14-21
FIGURE 7 – Structure of poly(w-alkenoic acid) carboxylates 25
One important surprise occurred when we recognized that the cause of the difference in the reactivity between methyl acrylate and higher methyl ω-alkenoates could be identiﬁed by the 13C NMR spectra of the methine carbon atom in the oleﬁn group of the ω-alkenoates and the oxirane methine carbon of the ω-alkanoate as well as the carbonyl carbon atom of the carboxylate group (Figure 10).28-33 The 13C NMR spectra showed remarkable chemical shift (δ) changes of the methine C-atoms and carbonyl carbons as methylene groups were added between the oleﬁnic double bond and the oxirane ring and the 17
carboxylate group. While the methine 13C NMR chemical shift value of ethyl glycidate was δ = 48, methyl 3-epoxybutenoate also δ = 48, methyl 4-epoxypentenoate was δ = 53 and methyl 5-epoxyhexenoate was also of d = 52.
functional carbomethoxy groups were separated by about 3 methylene spacers (Figure 11).
FIGURE 8 – The inﬂuence of the size of spacer group (n) on the rate of epoxidation of methyl ω-alkenoates30
FIGURE 11 – 13C NMR chemical shift values (δ) of methine carbons of oxirane and oleﬁn functional monomers33
FIGURE 9 – Structures of methyl ω-alkenoates and methyl ω-epoxyalkenoates monomers31
FIGURE 10 – 13C NMR chemical shift values (δ) of carbonyl carbons of oxirane and oleﬁne monomers depending on number of methylene groups32
The chemical shift values of epoxy esters with longer methylene spacer groups level off at about δ = 52, demonstrating the higher electron density on the methine carbon atom with increasing methylene groups shielding it from the carboxylate electron withdrawing effect (Figure 11). A similar effect was noticed with the chemical shift values of the 13 C NMR of the carbonyl carbon of the polymerizable groups when the 18
What was anticipated from the NMR spectra was also found when the appropriate esters of the ω-alkenoic acids and ω-epoxyalkanoic acids were subjected to polymerization. The polymerization rates were slower at the monomers with the lower monomeric esters and leveled out, when the side chain reached three methylene spacer units. From that point the ω-alkenoate esters acted like regular α-oleﬁns and the ω-epoxyalkanoates like regular epoxides. Polymer reactions Functional groups in polymers, when attached directly to the polymer chain have been known to react differently than functional groups in low molecular molecules. This different behavior had sometimes been called polymer effect. The question of the inﬂuence of the main polymer chain on the efﬁciency of substitution reaction certainly goes back to the study of hydrolysis of poly(methyl methacrylate).13 It became clear that the reactivity of these groups signiﬁcantly depended on how close they were to the polymer main chain and what reactions were involved. Some time ago, we undertook a careful study14-16,26-29 on the inﬂuence of the chain length between the functional group and the backbone chain. We have chosen methylene spacers and compared the more ﬂexible poly(oxy ethylene) with the polyethylene backbone chain. In the case of the poly(oxy ethylene) derivatives, it was found that the polymerizability of the w-epoxycarboxylate increased as the function of the methylene spacer length (n) increases17 and reaches a plateau after n-3. With the polyoleﬁn family, the polymerizability of α-oleﬁn carboxylate27 also increased, but it did not reach a plateau until one or two methylene spacer groups were added. Polymers of poly(oxy ethylene) and polyethylene esters were hydrolyzed to the corresponding ionomers and converted to the free polymeric acids. Studies were also undertaken to investigate the polyanion – polycation complex formation as a function of backbone ﬂexibility and side chain length.29 It is known how difﬁcult it was to hydrolyze poly(methyl methacrylate) quantitatively, how complicated it was to dehydrohalogenate PVC and how complicated it was to react poly(vinyl alcohol) with n-butyraldehyde quantitatively - and all that because of the dominating inﬂuence of the polymer chain. We have found that these problems can POLIMERI • 31 (2010) 1:14-21
be overcome, when polymers are used that have their reactive groups separated by ﬂexible methylene spacer groups of at least 3 carbon atoms from the main chain.34,35 We have used carboxylic acid derivatives to demonstrate this effect. Reactions are nearly quantitative, like reactions on low molecular weight compounds. We found that the most effective derivatives of ω-alkenoic acids and ω-epoxyalkanoic acids were their imidazolids, which react quantitatively with amines and phenols. For a quantitative conversion of aliphatic alcohols to the ester it is better to use the lithium alkoxide.34
H. Ringsdorf et al.39 investigated multilayered Langmuir-Blodgett ﬁlms of preformed polymers containing ﬂuorocarbon side chains and hydrophilic spacer groups in the main chain. Results indicate that the side chain is tilted relative to the surface normal unlike their hydrocarbon analogues, which are perpendicular to the surface. The contribution of the rigid ﬂuorocarbon side chain in this inherent thermal stability was discussed. The extent of orientation of the ﬂuorocarbon side chain was speciﬁcally addressed as a function of backbone spacer length and sample temperature.
Other polymer structures Fluorocarbon chemistry was energized when it was found that the ﬂuorooleﬁn group could be epoxidized. The most important compound that came out of this research was hexaﬂuoropropylene oxide.36 The signiﬁcant breakthrough took place in 1959 with the discovery of hexaﬂuoropropylene oxide. A whole new family of chemistry was developed around this discovery and led to important ﬂuorooleﬁn polymers. Copolymers with tetraﬂuoroethylene, became very important. The important comonomers were ﬂuorooleﬁns with a ﬂexible spacer side group of a hexaﬂuoropropylene oxide oligomer of about 2-3 oligomeric perﬂuorocarbon vinylethers groups terminated with sulfate ends on a tetraﬂuoroethylene backbone, usually at a ratio of 6:1.37 It was the basis for the later development of polyﬂuorosulfonic acids with the trademark Naﬁon (Figure 12). This copolymer was discovered by Walther G. Grot in the late 1960s and was the ﬁrst example of a ﬂuorocarbon ionomer. Soon thereafter the corresponding carboxylate terminated ﬂuoropolymers were commercialized.38 These two types of ﬂuorocarbon copolymers became the basis for the commercially important polyﬂuorocarbon sulfonates and carboxylates with the ﬂexible ﬂuorocarbon side chain.
Importance of spacers in initial polymerizations
FIGURE 12 – Structure of ionomere on the base of sulfonated ﬂuorocarbon (naﬁon)37
As it is well known, the isotactic polypropylene was discovered in the early 1950s by several groups using a transition metal catalyst consisting of TiCl3 with aluminum alkyls as modiﬁers.40 However, the primary credit goes to Natta and his research establishment.41 In 1957, Montecatini commercialized their invention. The polymerization was carried out in hexane as the solvent. This process produced about 104 g of polymer per milli-equivalent of the transition metal catalyst. Nearly 20 years later the so-called high yield catalyst systems based on the deposition of the transition metal catalyst onto magnesium chloride were discovered independently by Montedison in Italy and Mitsui Petrochemicals in Japan. This catalyst system produces 5x105 g polymer per milli-equivalent of transition metal. The largest factors to determine the stereo-regularity and of the polypropylene molecule are the deposition of the transition metal compounds on MgCl2 support and the use of electron donor compounds, which are considered to restrict the geometry of monomer coordination and polymer propagation (Figure 13a).42 In such a way, both the high stereoregularity and the high catalysts efﬁciency has been achieved. On the other hand, metallocene type catalysts have become commercially used recently. They stereoregularity is mostly determined by the ligand structure of the transition metal complex instead of the electron donor (Figure 13b).42 Montedison improved the high yield catalyst system for the propylene polymerization in 1982 into the Spheripol process,43 which is carried out in its initial stage in liquid propylene at 70ºC and 40 bars and ﬁnished in the gas phase. Further, recent improvement is the Borstar process. Here, the ﬁrst phase using TiCl3 and Al(C2H5)2Cl as the catalyst, the pre-polymerization is carried out in a loop reactor under supercritical conditions of about 90ºC and at pressures of about 50 bar followed by a second step in the gas phase. A different process, the gas phase process of propylene, is carried out directly in the gas phase at about 60-80°C. The propylene polymerization proceeds by inserting the monomer propylene by a coordinative process into the transition metal alkyl bond. After a few monomer units are inserted into the growing transitional metal bonded oligomer chain it crystallizes (Fig. 14). The question now is: at
FIGURE 13 – Stereoregularity control models of propylene polymerization by (a) Ziegler-Natta supported MgCl2 catalysts, (b) metallocene catalysts42
POLIMERI • 31 (2010) 1:14-21
what stage does crystallization occur and how many monomer units are needed for the stereospeciﬁc oligo-propylene chain to cause crystallization?18,44,45 Polypropylene as a crystalline 31 helical structure was ﬁrst determined by Corradini.44 He found it to be a helix with three monomer units per repeat unit of 0.56 nm and a turn angle of the helix of 120oC. The polypropylene, when molded from the melt crystallizes and melts at 165oC. Further investigations on polyethylene found that the polypropylene helices restructure into folded chains with a fold length of about 14 nm (about 25 repeat units). The folded chain was ﬁrst recognized in 1957.18 Polypropylene, like many crystalline helical polymers consists, for statistical reasons, of a 50:50 mixture of left and right-handed helices.
3. Kiliman, L. B., Deak, G., Vogl, O.: Liquid cristalline polymers of polyoleﬁn and poly (oxyethylene) derivatives, J. Macromol. Sci. Pure Appl. Chem., A38(2001)4, 329-352. 4. Zhou, D. et al.: Synthesis and properties of polyacetylenes containing terphenyl pendent group with different spacers, Macromolecules, 42(2009)5, 1454-1461. 5. Luckhurst, G.: Liquid crystals: a chemical physicist’s view, Liq. Crys., 32(2005)11-12, 1335-1364. 6. Anyanwu, U., Venkataraman, D.: Effect of spacers on the activity of soluble polymer supported catalysts for the asymmetric addition of diethylzinc to aldehydes, Tetrahedron Lett. 44(2003)6445–6448. 7. Pauling, L., Corey, R. B.: Conﬁguration of polypeptide chain with favored orientations around single bonds, Proc. Nat. Acad. Sci. USA, 37(1951)235. 8. Kauzman, W.: Some factors in the interpretation of protein denaturation, Adv. Protein Chem. 14(1959)1-63. 9. Bendu, D. A.: Denaturation of protein,. Dictionary of Food and Nutrition, 2005. 10. Tompa, P.: On the appearance and role of space group in the protein amino acids, J. Mol. Evol., 27(1988)147-153. 11. Vogl, O.: Polymerization of aliphatic aldehydes (1), J. Macromol. Sci., Chem. A, 1(1967)2, 243-266. 12. Vogl, O.: Polymerization of higher aldehydes, Adv. Chem. Ser., 52(1966)67.
FIGURE 14 – Simpliﬁed scheme of the beginning of polypropylene crystallization during coordinative polymerization reaction of propylene18
13. Wood, J. S., Negulescu, I., Vogl, O.: Higher aliphatic polyaldehydes. III. Crystal structure, crystallinity and melting transitions of isotactic poly(n-heptaldehyde), J. Macromol. Sci., Chem. A, 11(1977) (1), 171-194.
In the late 60s several groups studied the x-ray structure of native (as-prepared) isotactic polypropylene.46-49 Let us assume that the polymerization occurs completely stereospeciﬁcally and all additions are either levo (or dextro) as expected from statistical considerations. At what time crystallization occurs and how many monomer units are needed to begin the formation of the crystalline structure of a 31 helix?50 More importantly, does the polymer crystallization inﬂuence the stereochemistry of monomer addition at the monomer insertion stage? Isotactic polypropylene, crystallized from the melt,51 is a semi-crystalline polymer with a crystallinity of about 60% and a melt temperature (or point) of about 165oC.51 The crystal modiﬁcation has a repeat unit of 0.65 nm and consists of three phases (Figure 5): the α-phase (monoclinic) with a melt temperature of about 170oC, the β-phase (hexagonal) of about 155oC and the triclinic γ-phase52 for which several melt temperatures between 125oC and 150oC have been reported. The γ-phase crystallizes in the branching points of the spherulitic structure of the α-phase. The b-phase has to be nucleated and is not found in polypropylene, crystallized from the melt by spontaneous nucleation. The three phases differ from each other by slightly different arrangements of the left- and right-handed helices.
14. Negulescu, I., Vogl, O.: Higher aliphatic polyaldehydes. IV. Transitions in poly(nvaleraldehyde), poly (n-hexaldehyde), poly(n-heptaldehyde) and poly(n-octaldehyde), J. Polym. Sci., Polym. Chem. Ed., 14(1976)2995.
Conclusion The importance of short spacer groups on the crystallization of stereoregular polymer could possibly inﬂuence the stereospeciﬁcity of the addition to the catalyst site. From the information that we presented above - side chain polymerization of aliphatic polyaldehydes, polymerization of ω-alkenoates and knowing that isotactic polypropylene crystallizes in a 31 helix, we propose that the polypropylene chain as it is grows from the active catalyst, requires 6-8 monomer units in the amorphous state to be able to begin crystallizing into the crystalline 31 helical structure. It is not clear whether or not the glass transition temperature of polypropylene, which is about -5°C, should be taken into consideration in this argument, because this temperature has only the meaning for phases not for oligomers with few monomer units and all processes are carried out above this temperature. REFERENCES 1. Vogl, O.: Polymers with functional groups, Pure Appl. Chem., 51(1979), 2409-2419. 2. Vogl, O., Hatada, K., Kitayama, T. (Eds.): Macromolecular design of polymeric materials, Marcel Dekker Inc, New York, 1997.
15. Starr, J., Vogl, O.: Higher aliphatic aldehyde polymers. VII. Poly(n-decaldehyde), Monatsh. Chem., 109(1978)1241. 16. Starr, J., Vogl, O.: Higher aliphatic aldehyde polymers. 8. Poly(n-undecanal), Makromol. Chem., 179(1978)2621. 17. White J. I., Choi, D. D.: Polyoleﬁns - processing, structure development and properties, Hanser, Munnich, 2005. 18. Keller A.: A note on single crystals in polymers: evidence of a chain folded conﬁguration, Phil. Mag., 2(1957)1161. 19. Plate, N. A. et al.: Interphase interaction in heterogeneous polymeric systems containing liquid-crystalline component, Russ. Chem. Bull., 43(1994)1753-1769. 20. Janovic, Z. et al.: Lubricating oils pour point depressants based on alkyl methacrylate and styrene copolymers, Fuels Lubr. (Goriva i maziva), 45(2006)3, 143-163. 21. Vidović, E., Sarić, K., Janović, Z.: Copolymerization of styrene with dodecyl methacrylate and octadecyl methacrylate, Croat. Chem. Acta, 75(2002)3, 769-782. 22. Jukić, A. et al.: Terpolymerization kinetics of methyl methacrylate or styrene / dodecyl methacrylate / octadecyl methacrylate systems, Polym. Int., 56(2007)1, 112-120. 23. Šoljić, I., Jukić, A., Janović, Z.: Terpolymerization kinetics of N, N-dimethylaminoethyl methacrylate / alkyl methacrylate / styrene systems, Polym. Eng. Sci., 50(2010)3, 577-584. 24. Li, N. et al.: Synthesis and third-order NLO properties of polymethacrylates containing pendent azobenzene groups, High. Perform. Polym., 19(2007)3, 356-367. 25. Muggee, J., Vogl, O.: Poly(alkylene oxide) ionomers VIII. Synthesis of methyl ω-alkenoates and methyl ω-epoxyalkanoates, J. Polymer Sci., Polym. Chem. Ed., 22(1984)(10), 2501-2521. 26. Vogl, O.: Haloaldehyde polymers and macromolecular asymmetry, J. Polymer Sci., Polym. Chem. Ed., 38(2000)(15), 2623-2634. 27. Vogl, O., Muggee, J., Bansleben, D.: Poly(alkylene oxide) ionomers V. Polymers and copolymers of cyclic ethers with pendant carboxylate groups, Polym. J., 12(1980)9, 677-686. 28. Vogl, O. et al.: Polymers and copolymers of methyl ω-epoxyalkanoates. Part V of Poly(alkylene oxide) ionomers, in Coordination Polymerization (Eds. Price, C.C., Vandenberg, E.J.), Polym. Sci. Tech., 19(1983), 95-109. 29. Muggee, J., Vogl, O.: Poly(alkylene oxide) ionomers IX. Polymerization of methyl ω-epoxyalkanoates and characterization of the polymers, J. Polym. Sci., Part A: Polym. Chem., 24(1986)9, 2327-2349. 30. Vogl, O. et al.: Reactive groups, spacer groups and functional groups in macromolecular design, J. Macromol. Sci., Chem. A, 21(1984)8-9, 1217-1235. 31. Bansleben, D. A., Janović, Z., Vogl, O.: Poly(alkylene oxide) ionomers: XIII. Copolymers of trioxane with the epoxide and 1,3-dioxolane of methyl 10-undecenoate, J. Polym. Sci., Polym. Chem. Ed., 22(1984)11, 3263-3288. 32. Purgett, M. D., Vogl, O.: Functional polymers XLVIII. Polymerization of ω-alkenoate derivatives, J. Polymer Sci., Polym. Chem. Ed., 26(1988)3, 677-700.
POLIMERI • 31 (2010) 1:14-21
KATEGORIZIRANI RADOVI 33. Vogl, O.; Kiliman, L. B.: Poly(10,11-epoxyundecanoic acid), poly(5,6-epoxyhexanoic acid) and some of their derivatives, J. Macromol. Sci. Pure Appl. Chem. A, 38(2001)2, 123-135. 34. Deak, G., Vogl, O., Kiliman, L. B.: Poly(10-undecenoic acid) and some of its derivatives, J. Macromol. Sci. Pure Appl. Chem. A, 38(2001)3, 221-231. 35. Kiliman. L. B., Deak, G.; Vogl, O.: Liquid cristalline polymers of polyoleﬁn and poly(oxyethylene) derivatives, J. Macromol. Sci. Pure Appl. Chem. A, 38(2001)4, 329-352. 36. Resnick, P.: Perﬂuoroepoxides in Kirk Othmar Encyclopedia of Chemical Technology, Vol. 10, Third Edition, John Wiley, New York, 1980. 37. Mauritz, K. A., Moore, R. B.: State of understanding of naﬁon, Chemical Reviews 104(2004)4535. 38. Ukihashi, H., Yamabe, M., Miyake, H.: Polymeric ﬂuorocarbon acids and their applications, Progr. Polym. Sci., 12(1986)229. 39. Ringsdorf, J. et al.: Structural studies of polymers with hydrophilic spacer groups. 2. Infrared spectroscopy of Langmuir-Blodgett multilayers of polymers with ﬂuorocarbon side chains at ambient and elevated temperatures, Macromolecules, 22(1989)8, 3475-3480. 40. Moore, E. P.: Polypropylene Handbook, Hanser Verlag, New York, 1996. 41. Pino, P.: The impact of the discovery of the polymerization of the α-oleﬁns on the development of the stereospeciﬁc polymerization of vinyl monomers in Gulio Natta: Present Signiﬁcance of His Scientiﬁc Contribution (Eds: Carra, S., Parisi, F., Pasquon, I., Pino, P.), Edrice di Chimica Srl., 1982.
42. Muelhaupt, R.: Catalytic polymerization and post polymerization catalysis ﬁfty years after the discovery of Zieglers catalysts, Macromol. Chem. Phys., 204(2003)289-327. 43. Galli, P.: Methods of controlling morphology for tailoring polymer properties, the Spheripole process, J. Macromol. Sci. B, 35(1996)3, 427. 44. Natta, G., Corradini, P.: Structure and properties of isotactic polypropylene, Nuovo Cim. Suppl., 15(1960)40. 45. Bruckner, S., Meille, S. V.: Non-parallel chains in crystalline – isotactic polypropylene, Nature, 340(1969)455. 46. Blais, P., Manley, R.: Morphology of nascent Ziegler-Natta polymers, Science, 153(1966)539. 47. Wristers, J.: Nascent polypropylene morphology, J. Polym. Sci., Polym. Phys. Ed., 11(1973)8, 1601. 48. Guttman, J. Y.,Guillet, J. E.: Mechanism of propylene polymerization on single crystals of α-titanium trichloride, Macromolecules, 3(1970)4, 470. 49. Vogl, O., Jaycox, G.: Crystalline helical poymers, Polimeri, 18(1997)3-4, 141-149. 50. Vogl, O.: Polypropylene: an Introduction, J. Macromol. Sci. Pure Appl. Chem. A, 36(1999)11, 1547-1559. 51. Lotz, B., Wittman, J. C., Lovinger, A.: Structure and morphology of polypropylenes: a molecular analysis, Polymer, 37(1996)4979. 52. Bruckner, S., Meille, S. V.: non-parallel chains in crystalline γ-isotactic polypopylene, Nature, 340(1989)6233, 455-457.
CONTACT Dr. Otto Vogl Herman F. Mark Professor Emeritus Department of Polymer Science and Engineering University of Massachusetts Amherst, MA 01003-4350 U.S.A E-mail:[email protected]
Poziv na sudjelovanje na XXII. hrvatskom skupu kemičara i kemijskih inženjera Hrvatsko društvo kemijskih inženjera i tehnologa (HDKI) i Hrvatsko kemijsko društvo (HKD) organiziraju XXII. hrvatski skup kemičara i kemijskih inženjera, koji će se održati od 13. do 16. veljače 2011. u Zagrebu, u hotelu Four Points by Sheraton Panorama, pod pokroviteljstvom Sveučilišta u Zagrebu, Akademije tehničkih znanosti Hrvatske, Hrvatskoga inženjerskog saveza i Ministarstva zaštite okoliša i prostornog uređenja. Namjera ovoga skupa je predstavljanje znanstvene i stručne djelatnosti iz područja kemije, kemijskog inženjerstva i srodnih znanstvenih disciplina, s naglaskom na promicanju interdisciplinarnosti te primjeni znanosti u razvoju naprednih materijala, zaštiti okoliša i razvoju održivih tehnologija. Na skupu će se okupiti brojni znanstvenici i stručnjaci sa sveučilišta, istraživačkih instituta, iz škola i industrije iz Hrvatske i inozemstva. Predstavljanje najnovijih dostignuća i razmjena iskustava putem plenarnih i pozvanih predavanja, predavanja nagrađenih znanstvenika te usmenih i posterskih izlaganja najdjelotvorniji su načini širenja novih znanja, ideja i tehnologija radi doprinosa razvoju gospodarstva. Sva priopćenja održana na skupu bit će tiskana u Knjizi sažetaka. Kao pridružena manifestacija, uz skup će se održati izložba kemijskoga industrijskog i laboratorijskog POLIMERI • 31 (2010) 1:14-21
pribora i instrumentacije, računalne opreme i programske podrške te literature. Skup će raditi u sljedećim sekcijama: 1. Kemija 2. Kemijsko i biokemijsko inženjerstvo 3. Materijali 4. Obrazovanje 5. Zaštita okoliša 6. Dizajn kemijskih proizvoda. Detaljnije informacije o skupu mogu se naći na internetskoj stranici 22skiki.fkit.hr. Pozivamo vas da nam se pridružite na XXII. hrvatskom skupu kemičara i kemijskih inženjera te da svojim sudjelovanjem pridonesete njegovu uspjehu i kvaliteti. Predsjednica Znanstveno-organizacijskog odbora Vesna TOMAŠIĆ 21